Research Article  Open Access
SolvationAssisted Young’s Modulus Control of SingleCrystal Fullerene Nanowhiskers
Abstract
Singlecrystal nanowhiskers (NWs) composed of fullerene C_{70} molecules were synthesized by the liquidliquid interfacial precipitation method that used mxylene as a saturated solution of C_{70} molecules. Bending behavior of the individual NWs was observed by in situ transmission electron microscopy equipped with nanonewton force measurements using an optical deflection method. The Young’s modulus of the NWs was estimated to be 0.3–1.9 GPa, which was 2–7% of the moduli of fullerene NWs with similar diameters synthesized using other solvents, that is, toluene and pyridine. The influence of the solvent used in the precipitation method on Young’s modulus is discussed.
1. Introduction
Crystals composed of fullerene molecules have been synthesized by precipitation methods [1–13]. The crystals show various morphologies, that is, plates, films, and rods. In particular, Miyazawa et al. discovered the oneaxis preferential growth of fullerene single crystals; a liquidliquid interfacial precipitation (LLIP) method produces fullerene nanowhiskers (NWs) and nanotubes (NTs) with high lengthtodiameter aspect ratios [14]. Because this structural feature is suitable for application in advanced nanodevices, the mechanical properties of these NWs and NTs have been the focus of a considerable amount of research. In situ transmission electron microscopy (TEM) equipped with piezomanipulation of individual NWs and NTs enables investigating the mechanical properties of such nanometersized materials [15–18].
The Young’s moduli of fullerene NWs and NTs have been estimated by this method [19–22]. The structures of fullerene NWs and NTs synthesized by LLIP methods are influenced by solvation behaviors, suggesting that the mechanical properties depend on the solvents used. Two solvents, that is, toluene and pyridine, have been intensively used for the synthesis of NWs and NTs owing to their high productivity rates. In this study, we synthesized C_{70} NWs by the LLIP method using another solvent (mxylene) and investigated their mechanical properties by in situ TEM.
2. Experimental
A saturated solution of C_{70} molecules in mxylene was poured into isopropyl alcohol, followed by precipitation of C_{70} NWs. Then, the solution was added dropwise to an edge of a gold plate. The plate was mounted onto a specimen holder of the transmission electron microscope equipped with a piezomanipulation system at the University of Tsukuba [23–26]. A silicon microcantilever with a nanometersized tip that is used for contacttype atomic force microscopy was fixed onto a cantilever holder. Both the specimen and the cantilever holders were inserted in the microscope. The cantilever tip was brought into contact with individual NWs fixed on the plate edges by the piezomanipulation system of the microscope. The tip was then pressed on the NWs for bending with cantilever beamtype loading. The cantilever tip was then pulled back to release the force. A series of such manipulations was performed several times for the same NW at room temperature in a vacuum of Pa. The deformation process was observed in situ using a video capture system using a chargecoupled device camera with a time resolution of 17 ms. Simultaneously, the force applied on the NWs was measured by an optical detection of the cantilever deflection used in atomic force microscopy. The spring constant of the cantilever was measured to be 4.7 N/m.
3. Results
Figures 1(a)–1(c) show a timesequence series of the brightfield images of the bending process of a C_{70} NW protruding from an edge of the gold plate. The dark triangular region in the upper part of each frame is the cantilever tip. The brighter region around the NW is the vacuum. The outer diameter of the NW is 410 nm, and the length of the deformed portion is 1.2 μm. The crystal structure of the NT was tetragonal. This crystal structure has been observed in dried C_{60} NWs and NTs synthesized by LLIP methods [17–19]. This structure arises from polymerization of fullerene molecules [27]. The longer growth axis of the NW is aligned parallel to [110]. The left side of the NT in Figure 1 was fixed on the gold plate. In the bending test, the cantilever tip was initially placed in contact with the NW (Figure 1(a)). Then, the NT was pressed along the direction indicated by the arrow in Figure 1(a) to cause bending (Figure 1(b)). Subsequently, the tip was released, and the NT recovered its initial straight shape as in Figure 1(c). Thus, this bending behavior corresponds to an elastic deformation.
(a)
(b)
(c)
Figure 2 shows the relationship between the force and flexure during the bending process shown in Figure 1. The points indicated by arrowheads a–c in Figure 2 correspond to the TEM images in Figures 1(a)–1(c). The maximum flexure and loading at the free end were 300 nm and 1590 nN, respectively. Hysteresis is observed in the curve in Figure 2 during the pressing and pulling process of the cantilever tip. It is attributed to the bonding of the cantilever tip with the NW surface [28]. The curve of the pressing process (ab in Figure 2) can be approximated by one linear component. On the other hand, the curve of the pulling process (bc in Figure 2) is a sequence of several linear slopes. The slope of the pulling process near point c is similar to that of the pressing process. Thus, we used this slope for the estimation of the Young’s modulus of the NW. On the basis of the relationship among force, flexure, and Young’s modulus for cantileverbeam loading in standard mechanics of materials, the Young’s modulus of the NWs was estimated to be GPa. We performed bending tests with the same type of loading for other NWs with the outer diameters of 580 nm and 770 nm. Their Young’s moduli were estimated to be GPa and GPa, respectively.
Figure 3 shows the relationship between the Young’s modulus and the outer diameter of the C_{70} NWs. Note that the Young’s modulus increases as the outer diameter decreases. The relationship is well fitted by a straight line.
4. Discussion
The Young’s moduli of singlecrystal C_{60} and C_{70} particles, films, NWs, and NTs previously reported are shown in Table 1. The NWs and NTs in previous studies were synthesized by the LLIP method using toluene and pyridine as solvents. The Young’s modulus of the present C_{70} NWs synthesized by the LLIP method using mxylene is 0.3–1.9 GPa. Because the Young’s modulus of fullerene NWs depends on the outer diameter as shown in Figure 3 and in previous measurements [15, 17, 18], we compared the Young’s modulus of the present C_{70} NWs with that of C_{60} NWs with similar outer diameters. The Young’s modulus of the present C_{70} NW with an outer diameter of 410 nm is 7% of that of a C_{60} NW with an outer diameter of 420 nm. NTs have different structures from NWs, and the Young’s modulus of C_{60} NTs is ~220% higher than that of C_{60} NWs as shown in Table 1. The ratio of the modulus of C_{70} NWs to C_{60} NTs becomes further lower; the Young’s modulus of the C_{70} NW with an outer diameter of 580 nm is 2% of that of a C_{60} NT with an outer diameter of 510 nm. On the other hand, the modulus of the films in Table 1 indicates that by changing the constituent molecules from C_{60} to C_{70}, the modulus decreases only by 30–50%. This implies that the considerable decrease in the Young’s modulus of the present NWs cannot be attributed to only the difference in constituent molecules. Therefore, the decrease in the Young’s modulus in the present NWs is caused by the difference in solvents used in the LLIP.

During incubation, the crystal structures of fullerene NWs and NTs synthesized by the LLIP method using toluene and pyridine were investigated by Minato and Miyazawa [22]. Pristine NWs show solvated hexagonal structures that transform into facecentered cubic structures by desiccation. Thus, the solvents affect the molecular bonding, configuration, and defect formation in pristine NWs synthesized by LLIP methods. Strain, hollow spaces, or vacancycluster type defects are introduced when the molecules are disconnected by insertion of the solvents. It was also reported that stacking faults were formed in the fullerene crystals precipitated in oxylene [29]. As a result, these defects lead to the formation of pores in NWs after desiccation. In particular, the density of pores is higher in the interior region around the center axis [30]. Ringor and Miyazawa proposed that NTs are formed by elution of the interior regions with defects [31]. As Saito et al. discussed, the decrease in Young’s modulus of NWs with the outer diameter, which is observed in the present study, suggests the presence of defects in the interior regions [18]. The Young’s modulus of fullerene films decreases as density decreases [32, 33]. Therefore, it is deduced that the mxylene molecules remaining in the pristine NWs cause defects in the interior regions after desiccation, leading to the considerable decrease in Young’s modulus.
5. Conclusion
Using in situ TEM, we performed bending tests on individual singlecrystal C_{70} NWs synthesized by the LLIP method using mxylene as the solvent. The Young’s modulus of the NWs was estimated to be 0.3–1.9 GPa, which is 2–7% of the moduli of fullerene NWs and NTs with similar diameters synthesized using toluene and pyridine as solvents. It was inferred that the considerable decrease in Young’s modulus was caused by the higher number of defects in the interior regions introduced by solvation of mxylene in the pristine NWs. This result reveals that the Young’s modulus of NWs can be controlled to a doubledigit magnitude by appropriate selection of solvents, leading to design of structural materials using NWs.
Acknowledgment
This study was partly supported by GrantsinAid from the Ministry of Education, Culture, Sport, Science and Technology, Japan (nos. 22310065 and 23651127).
References
 W. Kratschmer, L. D. Lamb, K. Fostiropoulos, and D. R. Huffman, “Solid C_{60}: a new form of carbon,” Nature, vol. 347, no. 6291, pp. 354–358, 1990. View at: Publisher Site  Google Scholar
 W. I. F. David, R. M. Ibberson, J. C. Matthewman et al., “Crystal structure and bonding of ordered C_{60},” Nature, vol. 353, no. 6340, pp. 147–149, 1991. View at: Google Scholar
 S. J. Duclos, K. Brister, R. C. Haddon, A. R. Kortan, and F. A. Thiel, “Effects of pressure and stress on C_{60} fullerite to 20 GPa,” Nature, vol. 351, no. 6325, pp. 380–382, 1991. View at: Google Scholar
 P. A. Heiney, J. E. Fischer, A. R. McGhie et al., “Orientational ordering transition in solid C_{60},” Physical Review Letters, vol. 66, no. 22, pp. 2911–2914, 1991. View at: Publisher Site  Google Scholar
 R. L. Meng, D. Ramirez, X. Jiang et al., “Growth of large, defectfree pure C_{60} single crystals,” Applied Physics Letters, vol. 59, no. 26, pp. 3402–3403, 1991. View at: Publisher Site  Google Scholar
 W. Krakow, N. M. Rivera, R. A. Roy, R. S. Ruoff, and J. J. Cuomo, “Epitaxial growth of C_{60} thin films on mica,” Journal of Materials Research, vol. 7, no. 4, pp. 784–787, 1992. View at: Google Scholar
 X. D. Shi, A. R. Kortan, J. M. Williams, A. M. Kini, B. M. Savall, and P. M. Chaikin, “Sound velocity and attenuation in singlecrystal C_{60},” Physical Review Letters, vol. 68, no. 6, pp. 827–830, 1992. View at: Google Scholar
 Y. Yosida, “Scanning electron microscope images of C_{60} whiskers,” Japanese Journal of Applied Physics, vol. 31, no. 4 B, pp. L505–L507, 1992. View at: Google Scholar
 M. Haluška, H. Kuzmany, M. Vybornov, P. Rogl, and P. Fejdi, “A doubletemperaturegradient technique for the growth of singlecrystal fullerites from the vapor phase,” Applied Physics A, vol. 56, no. 3, pp. 161–167, 1993. View at: Publisher Site  Google Scholar
 J. Z. Liu, J. W. Dykes, M. D. Lan, P. Klavins, R. N. Shelton, and M. M. Olmstead, “Vapor transport growth of C_{60} crystals,” Applied Physics Letters, vol. 62, no. 5, pp. 531–532, 1993. View at: Publisher Site  Google Scholar
 J. L. de Boer, S. van Smaalen, V. Petricek, M. DusekP, M. A. Verheijen, and G. Meijer, “Hexagonal closepacked C_{60},” Chemical Physics Letters, vol. 219, no. 56, pp. 469–472, 1994. View at: Google Scholar
 F. Michaud, M. Barrio, S. Toscani et al., “Solidstate studies on single and decagonal crystals of C_{60} grown from 1,2dichloroethane,” Physical Review B, vol. 57, no. 17, pp. 10351–10358, 1998. View at: Google Scholar
 S. Toscani, H. Allouchi, J. L. Tamarit et al., “Decagonal C_{60} crystals grown from n hexane solutions: solidstate and aging studies,” Chemical Physics Letters, vol. 330, no. 56, pp. 491–496, 2000. View at: Google Scholar
 K. Miyazawa, A. Obayashi, and M. Kuwabara, “C_{60} nanowhiskers in a mixture of lead zirconate titanate solC_{60} toluene solution,” Journal of the American Ceramic Society, vol. 84, no. 312, pp. 3037–3039, 2001. View at: Google Scholar
 K. Asaka, R. Kato, K. Miyazawa, and T. Kizuka, “Buckling of C_{60} whiskers,” Applied Physics Letters, vol. 89, no. 7, Article ID 071912, 2006. View at: Publisher Site  Google Scholar
 R. Kato, K. Asaka, K. Miyazawa, and T. Kizuka, “In situ highresolution transmission electron microscopy of elastic deformation and fracture of nanometersized fullerene C_{60} whiskers,” Japanese Journal of Applied Physics, vol. 45, no. 10 A, pp. 8024–8026, 2006. View at: Publisher Site  Google Scholar
 T. Kizuka, K. Saito, and K. Miyazawa, “Young's modulus of crystalline C_{60} nanotubes studied by in situ transmission electron microscopy,” Diamond and Related Materials, vol. 17, no. 6, pp. 972–974, 2008. View at: Publisher Site  Google Scholar
 K. Saito, K. Miyazawa, and T. Kizuka, “Bending process and Young's modulus of fullerene C_{60} nanowhiskers,” Japanese Journal of Applied Physics, vol. 48, no. 1, Article ID 010217, 2009. View at: Publisher Site  Google Scholar
 K. Miyazawa, “C_{70} nanowhiskers fabricated by forming liquid/liquid interfaces in the systems of toluene solution of C_{70} and isopropy/alcohol,” Journal of the American Ceramic Society, vol. 85, no. 5, pp. 1297–1299, 2002. View at: Google Scholar
 K. Miyazawa, K. Hamamoto, S. Nagata, and T. Suga, “Structural investigation of the C_{60}/C_{70}whiskers fabricated by forming liquidliquid interfaces of toluene with dissolved C_{60}/C_{70} and isopropyl alcohol,” Journal of Materials Research, vol. 18, no. 5, pp. 1096–1103, 2003. View at: Google Scholar
 K. Miyazawa, Y. Kuwasaki, K. Hamamoto, S. Nagata, A. Obayashi, and M. Kuwabara, “Structural characterization of C_{60} nanowhiskers formed by the liquid/liquid interfacial precipitation method,” Surface and Interface Analysis, vol. 35, no. 1, pp. 117–120, 2003. View at: Publisher Site  Google Scholar
 J. I. Minato and K. Miyazawa, “Structural characterization of C_{60} nanowhiskers and C_{60} nanotubes fabricated by the liquidliquid interfacial precipitation method,” Diamond and Related Materials, vol. 15, no. 48, pp. 1151–1154, 2006. View at: Publisher Site  Google Scholar
 T. Kizuka, K. Yamada, S. Deguchi, M. Naruse, and N. Tanaka, “Crosssectional timeresolved highresolution transmission electron microscopy of atomicscale contact and noncontacttype scannings on gold surfaces,” Physical Review B, vol. 55, no. 12, pp. R7398–R7401, 1997. View at: Google Scholar
 T. Kizuka, “Atomic process of point contact in gold studied by timeresolved highresolution transmission electron microscopy,” Physical Review Letters, vol. 81, no. 20, pp. 4448–4451, 1998. View at: Google Scholar
 T. Kizuka, “Direct atomistic observation of deformation in multiwalled carbon nanotubes,” Physical Review B, vol. 59, no. 7, pp. 4646–4649, 1999. View at: Google Scholar
 T. Kizuka, “Atomic configuration and mechanical and electrical properties of stable gold wires of singleatom width,” Physical Review B, vol. 77, no. 15, Article ID 155401, 2008. View at: Publisher Site  Google Scholar
 A. V. Soldatov, G. Roth, A. Dzyabchenko et al., “Topochemical polymerization of C_{70} controlled by monomer crystal packing,” Science, vol. 293, no. 5530, pp. 680–683, 2001. View at: Google Scholar
 S. Fujisawa and T. Kizuka, “Effect of lateral displacement of atomic force microscope tip caused by contact scanning studied by in situ transmission electron microscopy,” Japanese Journal of Applied Physics, vol. 42, no. 10 A, pp. L1182–L1184, 2003. View at: Google Scholar
 M. Gu and T. B. Tang, “Thermoanalytical studies on the orderdisorder transition in C_{60} doped with C_{70},” Journal of Physics: Condensed Matter, vol. 7, no. 38, pp. 7475–7479, 1995. View at: Publisher Site  Google Scholar
 R. Kato and K. Miyazawa, “Crosssectional structural analysis of C_{60} nanowhiskers by transmission electron microscopy,” Diamond and Related Materials, vol. 20, no. 3, pp. 299–303, 2011. View at: Publisher Site  Google Scholar
 C. L. Ringor and K. Miyazawa, “Fabrication of solution grown C_{60} fullerene nanotubes with tunable diameter,” Journal of Nanoscience and Nanotechnology, vol. 9, no. 11, pp. 6560–6564, 2009. View at: Publisher Site  Google Scholar
 A. A. Kolomenskii, M. Szabadi, and P. Hess, “Laser diagnostics of C_{60} and C_{70} films by broadband surface acoustic wave spectroscopy,” Applied Surface Science, vol. 86, no. 1–4, pp. 591–596, 1995. View at: Publisher Site  Google Scholar
 P. Murugavel, C. Narayana, A. Govindaraj, A. K. Sood, and C. N. R. Rao, “Brillouin scattering from C_{70} and C_{60} films: a comparative study of elastic properties,” Chemical Physics Letters, vol. 331, no. 2–4, pp. 149–153, 2000. View at: Google Scholar
 S. Hoen, N. G. Chopra, X. D. Xiang et al., “Elastic properties of a van der Waals solid: C_{60},” Physical Review B, vol. 46, no. 19, pp. 12737–12739, 1992. View at: Publisher Site  Google Scholar
 N. P. Kobelev, R. K. Nikolaev, Y. M. Soifer, and S. S. Khasanov, “The elastic stiffness matrix of singlecrystal C_{60},” Chemical Physics Letters, vol. 276, no. 34, pp. 263–265, 1997. View at: Google Scholar
 D. Fioretto, G. Carlotti, G. Socino et al., “Brillouinscattering determination of the elastic constants of epitaxial fcc C_{60} film,” Physical Review B, vol. 52, no. 12, pp. R8707–R8710, 1995. View at: Publisher Site  Google Scholar
 H. Coufal, K. Meyer, R. K. Grygier, M. de Vries, D. Jenrich, and P. Hess, “Measurement of the elastic properties of evaporated C_{60} films by surface acoustic waves,” Applied Physics A, vol. 59, no. 1, pp. 83–86, 1994. View at: Publisher Site  Google Scholar
 T. Kizuka, K. Miyazawa, and T. Tokumine, “Young's modulus of singlecrystal fullerene C_{70} nanotubes,” Journal of Nanotechnology, vol. 2012, Article ID 969357, 5 pages, 2012. View at: Publisher Site  Google Scholar
Copyright
Copyright © 2012 Tokushi Kizuka et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.